Correction to Structural Phase Transitions in EuC2
Derk Wandner; Pascal Link; Oliver Heyer; John Mydosh; Mahmoud A. Ahmida; Mohsen M. Abd-Elmeguid; Manfred Speldrich; Heiko Lueken; Uwe Ruschewitz; Inorganic Chemistry 50 (2011) 2703–2703; doi:10.1021/ic200013z

data_4324732
_publ_section_title
;
 Correction to Structural Phase Transitions in EuC2
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2703
_journal_page_last               2703
_journal_paper_doi               10.1021/ic200013z
_journal_volume                  50
_journal_year                    2011
_chemical_formula_sum            'C2 Eu'
_chemical_formula_weight         175.98
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_audit_author_name               EuC2_648
_audit_creation_date             2010-11-19T15:25
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2010-11-19T15:25  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   6.1379(4)
_cell_length_b                   6.1379
_cell_length_c                   6.1379
_cell_measurement_temperature    648
_cell_volume                     231.238(15)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      648
_diffrn_radiation_polarisn_ratio 0.95
_diffrn_radiation_probe          x-ray
_diffrn_radiation_wavelength     0.470257
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_pd_block_id                     2010-11-19T15:25|EUC2_648_phase1|EuC2_648||
_pd_calc_method                  'Rietveld Refinement'
_pd_phase_name                   EuC2
_pd_proc_info_datetime           2010-11-19T15:25:21
_pd_proc_ls_background_function
;   GSAS Background function number 7 with  9 terms.
 Linear interpolation
      1:    3382.43     2:    2700.02     3:    2772.61     4:    2805.95    
      5:    2372.12     6:    1854.29     7:    1667.25     8:    1448.26    
      9:    1434.10    
;
_pd_proc_ls_prof_R_factor        0.0954
_pd_proc_ls_prof_wR_expected     0.0188
_pd_proc_ls_prof_wR_factor       0.1239
_refine_ls_goodness_of_fit_all   6.61
_refine_ls_matrix_type           full
_refine_ls_number_parameters     19
_refine_ls_number_restraints     1
_refine_ls_R_Fsqd_factor         0.32051
_refine_ls_shift/su_max          0.08
_refine_ls_shift/su_mean         0.01
_reflns_d_resolution_high        0.690
_reflns_d_resolution_low         3.544
_reflns_limit_h_max              9
_reflns_limit_h_min              1
_reflns_limit_k_max              6
_reflns_limit_k_min              0
_reflns_limit_l_max              5
_reflns_limit_l_min              0
_reflns_number_total             57
_cod_data_source_file            ic200013z_si_003.cif
_cod_data_source_block           EUC2_648_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to the
built-in table from CIF Core dictionary named 'cif_core.dic' version
2.4.1 from 2010-06-29 (24 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        231.24(5)
_cod_original_formula_sum        'C2.00 Eu'
_cod_database_code               4324732
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000